Rochester Institute of Technology
RIT Scholar Works
Theses Thesis/Dissertation Collections
The integration of Si-based resonant interband
Follow this and additional works at:http://scholarworks.rit.edu/theses
This Thesis is brought to you for free and open access by the Thesis/Dissertation Collections at RIT Scholar Works. It has been accepted for inclusion in Theses by an authorized administrator of RIT Scholar Works. For more information, please firstname.lastname@example.org.
The Integration of Si-based Resonant Interband
Tunnel Diodes with CMOS
A Thesis Submitted
in Partial Fulfillment
of the Requirements for the Degree of
Master of Science
Dr. Santosh K. Kurinec (Thesis Advisor)
Dr. Sean L. Rommel (Committee)
Dr. Karl D. Hirschman (Committee)
Dr. Paul. R. Berger (External Collaborator) Dr. Phillip E. Thompson (External Collaborator)
DEPARTMENT OF MICROELECTRONICS ENGINEERING
COLLEGE OF ENGINEERING
ROCHESTER INSTITUTE OF TECHNOLOGY
A tribute of love to my parents,
Johan and Febiana
for the love, encouragements,
This work is a team effort. The successful completion of this thesis was made
possible through the generous support of Dr. Santosh K. Kurinec, who not only provided
the necessary vision and direction but also continuously gave encouragement and morale
support. I would also like to thank Dr. Sean L. Rommel for his inspiring leadership. His
knowledge on tunnel diodes, consistency, superb communication skill, and positive
influence have propelled this project into higher level. My deep appreciation also goes to
Dr. Karl D. Hirschman whom persistence and tireless effort in providing a reliable
baseline CMOS process have made this project successful.
I also would like to express my gratitude to Dr. Phillip E. Thompson of the Naval
Research Lab, Washington, D.C., for growing the tunnel diode layers. He was literally
the backbone of the entire project. I also thank Dr. Paul R. Berger, who is the principal
investigator of this research project funded by National Science Foundation (NSF,
ECS-0196054), and his graduate student Niu Jin at Ohio State University, Columbus, OH, for
their support in providing the RITD design template and performing post-growth thermal
Furthermore, I would like to thank my colleagues, Rohit Nandgaonkar, Branislav
Curanovic, Jeremiah Hebding, Robert Saxer, Keith Tabakman, Samantha Banker, Jeremy
Kempisty, and Andrew Estroff for their contributions in the mask design, process
qualification, and fabrication.
The completion of this project would not be possible without the generous support
David Yackoff, Sean O’Brien, and John Nash. Special thanks go to Jeffrey Peterson
who has trained me in most the tools needed for this project.
I would like to say my appreciation for some of my friends who have been
faithful in supporting me with their prayers and love: Renee, Jim and Louise, Yat-Wei
and Fook-Nee, David and Marie, and Eldon. Finally, I would like to give thanks to my
The first demonstration of the integration of CMOS and Si/SiGe resonant
interband tunnel diode (RITD) is reported in this study. RTD-FET circuits in III-V
materials have demonstrated improved speed and power capability in electronic circuits.
In Si-based material, recent breakthrough in Si/SiGe RITD grown using molecular beam
epitaxy (MBE) made the integration with CMOS possible. Discrete Si/SiGe RITDs
typically exhibit a PVCR of 3.6 and Jp of 0.3 kA/cm2.
The CMOS devices used in this study features (1) double-well technology, (2)
localized oxidation on silicon (LOCOS) to provide isolation between devices, (3) SiO2
gate dielectric of 370 Å thick, (4) highly n-doped polysilicon gate, (5) self-aligned source
and drain formation, and (6) Al doped with Si for contact and metallization. Based on
thermal budget considerations, the strategy employed was to integrate the RITD after all
CMOS high thermal front-end steps, up to the source/drain formation, but prior to
metallization. The tunnel diodes were grown through openings in a 300 nm-thick
chemical vapor deposition (CVD) oxide. The RITDs were also grown a top of p+
implanted regions of the source and drain of the PMOS. Process integration challenges
studied in this work include the effect of pre-growth substrate cleaning, patterned growth
and overgrowth methods, and residual implant damage.
Si/SiGe RITDs grown by MBE have been monolithically integrated with CMOS
for the first time. The integrated devices resulted in a PVCR of 2.8 and Jp of 0.3 kA/cm2
at room temperature, which enables the realization of RITD/CMOS circuitry. For the
first time, a NMOS-RITD MOBILE latch was demonstrated in Si. This logic element
Title Page ……… i Acknowledgement ………. iii Abstract ………..………..………..…..……..……… v Table of Content ………..………..………..………..………..………..……..…..…. vi List of Figures ………..………..………..………..………..………..….……..…… ix List of Tables ………..………..………..………..………..………..…………...….. x
1. Introduction and Motivation ………..………..………..………..………….…… 1
1.1. Tunnel Diode Benchmarks ………..………..………..……… 2
1.2. RTD-FET for Logic and Memory Applications ………..………..……..…. 4
1.3. Organization of Thesis ………..………..………..……..…..………..……. 6
2. Tunnel Diodes ………..………..………..………..………..…………. 7
2.1. Quantum Mechanical Tunneling ………..………..………..………..……. 7 2.2. Esaki Tunnel Diodes ………..………..………..………..………..……… 10 2.3. Resonant Tunnel Diodes ………..………..………..………..………..….. 15 2.4. Resonant Interband Tunnel Diodes ………..………..………..………….. 18 3. Silicon Based Resonant Interband Tunnel Diodes ………..………..………..… 20 3.1. Historical Development ………..………..………..………..………..…… 20
3.2. Fabrication Processes and Challenges ………..………..………..……….. 25
3.2.1. Substrate Cleaning and Preparation ………..………..………..….. 25 3.2.2. Low Thermal Molecular Beam Epitaxy ………..………..………. 26 3.2.3. Post-growth Rapid Thermal Anneal ………..………..………..…. 30
3.2.4. Patterning and Metallization ………..………..………..…………. 32
5. Process Integration Challenges and Their Effects on
RITD Device Characteristics …... 49 5.1. Process Integration Challenges ………..………..………..………..…..… 49 5.2. Experimental Details ………..………..………..………..………..……… 53 5.3. Experimental Results ………..………..………..………..………..……… 54 5.4. Analysis of RITD Device Characteristics ………..………..………..……. 57 5.4.1. The Effect of Patterned Growth ………..………..………..……... 57 5.4.2. The Effect of Residual Implant Damage ………..………..……… 58 5.4.3. The Effect of Sintering ………..………..………..………..……... 59 6. Study on Geometry and Area Dependence ………..………..………..………... 61 6.1. Defining The Area of RITD ………..………..………..………..………... 61 6.2. Design of Experiment ………..………..………..………..………..……... 62 6.3. Experimental Result and Analysis ………..………..………..………..…. 63 6.3.1. The Effect of Area on Series Resistance ………..………..……… 63 6.3.2. The Effect of Area on Jp, Jv, and PVCR ………..………..………. 66
6.3.3. The Effect of Geometry on Device Performance ………..………. 69 6.3.4. The Effect of Contact Cut Area on Series Resistance ………..….. 70 7. Overgrowth RITD ………..………..………..………..………..………..……… 72 7.1. The Problem of Misalignment ………..………..………..………..……… 72 7.2. Overgrowth RITD Structure ………..………..………..………..………... 74 7.3. Preliminary Experiment ………..………..………..………..………..…… 75 7.4. Result and Analysis ………..………..………..………..………..……….. 76
7.4.1. Current-Voltage Characteristics ………..………..………..……... 76
7.4.2. Scalability and Area Dependence ………..………..………..…… 80 7.4.3. Optimum Design ………..………..………..………..………..….. 82 8. Monolithic Integration of CMOS with Si/SiGe Resonant
Table Description Page
2.1. Examples of reported Esaki tunnel diode results for various materials. The entries listed in the table list the highest reported experimental values in each system. Adopted from Rommel .
2.2. Examples of reported RTD results for various materials. The entries listed in the table list the highest reported experimental values in each system.
2.3. Examples of reported RITD results for various materials. RITD type refers to configurations defined by Sweeny. Adopted from Rommel .
3.1. Chronological development of RITD technology. 24
3.2. Abbreviated Shiraki cleaning process develop at Naval Research Laboratory. Adopted from Thompson .
3.3. LT-MBE process to fabricate SiGe RITD structure as described in Fig. 3.3 (a). Process recipe is courtesy of Phillip E. Thompson.
4.1. Thermal budget of CMOS and RITD. The CMOS process is based on the twin-well CMOS technology developed at Rochester Institute of Technology.
4.2. RITD-CMOS testchip mask levels. Two additional mask levels were
added to incorporate RITD on to CMOS. 43
4.3. RITD-CMOS step-by step process. 44
4.4. Modified coating-to-development recipe to overcome resist adhesion problem.
5.1. Processes and structural differences between discrete device and
RITD built on CMOS platform. 50
5.2. Device structure schematics and electrical performance. 56
6.1. Processes and structural differences between discrete device and RITD built on CMOS platform.
Fig. Caption Page
1.1. Emerging Technology Sequence. Adopted from 2001 ITRS . 2
1.2. Current-Voltage (I-V) characteristic of a typical tunnel diode. Adopted from Sze .
1.3. Schematic diagram of an RTD-MODFET comparator circuit vs. a MODFET-only comparator circuit, comparators designed for 35 GHz operation, indicating the reduction in component count and
improvement in circuit speed. Adopted from Seabaugh .
1.4. The schematic circuit diagram and I-V characteristic of a T-SRAM memory cell. Adopted from van der Wagt .
2.1. Schematic diagram showing the tunneling of an electron or similar particle from the left of the potential barrier of thickness L and height V0, which is greater than the incident particle energy. Adopted from
2.2. (a) Triangular potential barrier; (b) parabolic potential barrier. Adopted from Sze .
2.3 Schematic energy diagram of Esaki tunnel diode. Adopted from Sze . 10
2.4. Schematic energy band diagram of tunnel diode in: (a) reverse bias; (b) thermal equilibrium or zero bias; (c) to (d) different stages of forward bias conditions; (e) the corresponding I-V characteristic.
2.5. Three current components of static I-V characteristic of tunnel diode: band-to-band tunnel current, excess current, and thermal current. Adopted from Sze .
2.6. Mechanism of tunneling via states in the forbidden gap for the excess current flow. Adopted from Chynoweth .
2.7. A potential well of finite width and depth. Electron bound within the well have discrete energies. Adopted from Hummel .
2.8. (a) RTD at zero bias. (b) Small forward bias is applied, creating
resonance condition so that tunneling occurs. (c) Biasing beyond critical voltage results in NDR behavior. (d) The corresponding static IV
characteristic. Adopted from McKelvey .
2.9. Schematic energy band diagram of proposed RITD. Heterojunctions forms quantum wells on conduction and valence bands. Adopted from Sweeny and Xu .
2.10. (a) Schematic band diagram of a modulation-doped RITD. Quantum well on both side of the diode can be formed using two delta planes. Adopted from Sweeny . (b) Discrete energy levels in δ-doped plane. Adopted from Gossmann .
3.1. Schematic diagram of the first Si/SiGe/Si RITD structures. (a)
Tunneling barrier was 4 nm Si0.5Ge0.5. (b) Additional 1 nm of undoped
on either side of Si0.5Ge0.5 was utilized as tunneling barrier. (c) The
schematic energy band diagram of structure TD2. (d) IV-characteristic of TD2. Adopted from Rommel .
3.2. (a) IV characteristic of different annealing temperature for structure consisting δB/3nm Si0.54Ge0.46/1 nm Si/δP. (b) The corresponding Jp, Jv,
and PVCR. Adopted from Eberl .
3.3. (a) Schematic diagram of RITD with SiGe cladding layers to suppress B diffusion. (b) Schematic energy band diagram of the corresponding structure. (c) The solid line represents the IV characteristic of structure in (a). Adopted from Niu .
3.4. Atomic sites in a simple cubic crystal. Adopted from Ghandhi . 27
3.5. Basic configuration of an MBE tool. Adopted from Ghandhi . 28
3.6. Schematic diagram of typical RTA system. Adopted from Ghandhi . 31
3.7. (a) The suppression of boron diffusion during post-growth anneal utilizing SiGe cladding layer. (b) The optimum anneal conditions for different RITD structures. Adopted from Jin .
4.1. Schematic diagram of RITD built right on top of S/D of FET device. Adopted with modification from Seabaugh .
4.2. RITD grown on regions that have been implanted with identical condition as P+S/D of PMOS.
4.3. The layout design of RITD-CMOS testchip. The die size is 5000 µm by 5000 µm.
4.4. The schematic layout of (a) PMOS and (b) NMOS with different channel dimensions from L = 2 µm x 32 µm to L=16 µm x 32 µm.
4.5. The schematic layout of (a) CMOS inverter of different gains, and (b)
CMOS ring oscillator. 39
4.6. The schematic layout of (a) square, (b) octagonal, and (c) circular RITDs. The size of these tunnel diodes ranges from 10 µm to 100 µm in diameter.
4.7. The schematic layout of a TSRAM cell. 41
4.9. The schematic layout of (a) resistors, (b) comb structures, (c) Van der
Pauw, and (d) Cross-Bridge Kelvin Resistors (CBKR). 42
4.10. The schematic layout of (a) resolution and alignment veneers, and (b) GCA alignment star.
4.11. Top View photograph of resist on top of MBE grown layer: (a) After coating using SVG Track standard recipe, i.e. at 4500 rpm, (b) After coating using manual spinner at 4000 rpm, (c) After development, showing resist pilling-off the surface, and (d) After coating at 2700 rpm, exposure, and development.
5.1. Schematic comparison between (a) discrete RITDs and (b) monolithically integrated RITDs on CMOS platform.
5.2. Schematic of (a) selective or preferential growth as in the vapor phase epitaxy and (b) patterned growth utilized in this study.
5.3. Anneal characteristic of boron in silicon. 52
5.4. Aluminum spikes creating a conducting path and shorting device. 52
5.5. PVCR distribution on patterned growth RITD on p+ implanted regions. 54
5.6. RITD Current-Voltage characteristics of different structures. 56
5.7. Scanning Electron Microscope (SEM) micrograph of MBE layers grown in an oxide opening. (Courtesy of Peter Terrana, RIT).
5.8. TEM Micrograph of RITD layers grown atop of implanted regions. The residual implant damage propagates through RITD layers. (Courtesy of Dr. Amitabh Jain of Texas Instrument).
5.9. RITD Current-Voltage characteristics of different sintering times. The inset shows the shift of peak voltage and PVCR with time.
6.1. RITD Area is defined as the size of the mesa structure shown in shaded
area. Different geometry: (a) square, (b) circle, and (c) octagonal. 61 6.2. Current-Voltage characteristics of square patterned growth RITDs on p+
implanted regions with different device sizes.
6.3. Schematic diagram of (a) current path in RITD that illustrates current crowding and spreading phenomenon, and (b) the effect of scaling in current density in vertical and horizontal direction.
6.4. Peak-to-valley current ratio as a function of area for different device
6.5. Peak current density (Jp) as a function of area for different device
6.7. PVCR of patterned growth RITDs on p+ substrate as a function of area
for different geometries. 69
6.8. Current-Voltage characteristics of 25 µm2 patterned growth RITDs on p+ substrate with different contact sizes.
7.1. Schematic diagram of metal short-circuits RITD junctions due to
mesa-to-contact cut misalignment. 73
7.2. Schematic diagram of metal short-circuits RITD junctions due to mesa-to-contact cut misalignment.
7.3. Cross-sectional diagram of an ideal overgrowth RITD that utilizes different crystalline structures to provide self-aligned process.
7.4. Cross-sectional diagram of overgrowth RITD. 75
7.5. Current-Voltage characteristics of 31/25/19 patterned growth and 31/37/31 overgrowth RITD. The secondary y-axis shows the difference between these two currents.
7.6. (a) Top-view diagram of superimposed layout of 31/25/19 patterned growth and 31/37/31 overgrowth RITD. (b) Circuit diagram if region A, B, and C are all behaving as tunnel diodes. (c) Circuit diagram if only region A and B are acting as tunnel diodes, and region C as resistor, providing device isolation around the active device region.
7.7. Peak current density vs. bias voltage for 31/25/19 patterned growth and
31/37/31 overgrowth RITD. 79
7.8. PVCR as a function of area for patterned and overgrowth RITD. 80
7.9. Jp as a function of area for patterned and overgrowth RITD. 81
7.10. Jv as a function of area for patterned and overgrowth RITD. 81
7.11. Top-view diagram of overgrowth RITD with a hypothetical line that separates the crystalline and non-crystalline regions.
7.12. PVCR, Jp, and Jv as a function of R-value. Below the optimum
condition, represented by the dashed line, defects in region B dominates device performance. Beyond the optimum R-value, defects in region A dominates.
7.13. PVCR versus R-value for different values of d. The inset shows that the optimum R-values decays exponentially with increasing values of d.
8.1. Schematic cross-sectional diagram of RITD/CMOS. 86
8.2. The ID-VD characteristics of PMOS and NMOS with Leff of 1.5 µm and
width of 32 µm.
8.3. Current-Voltage characteristics of a 25 × 25 µm2 patterned growth RITD grown on the same die as CMOS devices.
8.4. Different latches configurations: (a) a single RITD in series with a resistor, (b) a pair of RITDs with a resistive load, (c) MOBILE latch, and (d) NMOS-RITD MOBILE latch.
8.5. Current-voltage characteristics of RITD in series with different load resistors. Beyond the critical RL value, the tunnel diode exhibit
8.6. A current-voltage analysis of tunnel diode when (a) RL = 0 Ω, (b) RL <
RL(critical), (c) RL = RL(critical), and (d) RL > RL(critical).
8.7. Current-Voltage characteristics of two 25 × 25 µm2 RITDs in series with PVCR of 2.76 and 2.57, and Jp of 0.257 kA/cm2.
8.8. Voltage at sense node (VSN) as a function of supply voltage (VDD) of a
pair of RITDs in series with (a) RL of 180 Ω, (b) RL of 300 Ω, and (c)
RL of 600 Ω.
8.9. Voltage response at sense node (VSN) versus supply voltage of a pair of
RITDs in series with RL of 600 Ω, and the corresponding load line for
different supply voltage conditions.
8.10. Current-voltage characteristics of MOBILE latch configuration with different values of IIN.
8.11. Voltage response at sense node (VSN) as a function of supply voltage of
a MOBILE latch for different values of IIN.
8.12. MOBILE latch that exhibits ~ 100% voltage swing. 99
8.13. Current-Voltage characteristics of a NMOS-RITD MOBILE latch for different gate bias voltages.
8.14. Voltage response at sense node (VSN) as a function of supply voltage of
a NMOS-RITD MOBILE latch for different gate bias voltages.
8.15. Percentage of voltage swing as a function of the applied voltage supply for different gate bias voltages.
The rapid growth in microelectronics and computer industry has been fueled by
the rigorous effort of scaling down CMOS device dimensions. The printed gate length of
a transistor is often used as a benchmark that defines the technology node. Today’s state
of the art industries are capable of delivering transistors with gate length of 100 nm,
while developing the next generation devices towards the 65 nm technology node. This
conventional CMOS device, however, will begin to meet very challenging scaling efforts
as it approaches gate linewidth of about sub 70 nm. The limitation is not due to the
inability to shrink its physical dimension, but due to some quantum phenomena effects
that begin to dominate the device operation. Tunneling through ultra thin gate oxides and
extremely narrow channels results in an unacceptably high leakage current, which
significantly increases the static power dissipation. The fluctuation of the number of
dopant atoms in the channel regions that is only few atoms wide creates wide operating
margins from one transistor to another [1-3].
The 2001 edition of International Technology Roadmap for Semiconductors
(ITRS) predicted several emerging technologies that can provide near-term or low-risk
solutions, and one of these is the RTD-FET (Resonant Tunneling Diodes – Field Effect
Transistors) technology , which is the focus of this study.
The incorporation of tunnel diodes into any FET technology is expected to
significantly enhance circuit performance: higher circuit speed, reduced component
count, and lowered power consumption. The technology, however, is not intended to
Figure 1.1: Emerging Technology Sequence. Adopted from 2001 ITRS .
1.1. Tunnel Diode Benchmarks
The current-voltage characteristic of tunnel diode exhibits a unique negative
differential resistance (NDR) behavior as shown in Fig. 1.2. Quantum mechanical
tunneling is readily observed at a low forward-bias condition, resulting in a sudden rise in
current. The NDR originates from abrupt changes in the probability of tunneling through
potential barrier as the diode biased beyond critical voltage called the peak voltage (Vp).
The decrease in current continues until the second critical voltage known as valley
Figure 1.2: Current-Voltage (I-V) characteristic of a typical tunnel diode. Adopted from Sze .
The most important parameter used to characterize the performance of tunnel
diodes is the peak-to-valley current ratio (PVCR). The PVCR will always be greater than
1, and substantially larger values are desirable. It is defined by the following equation.
where Ip is the peak-current, and Iv is the valley current. Often these numbers are expressed in terms of current density, peak current density (Jp), and valley current density (Jv). Depending upon the application, Jp is often quoted as another important benchmark of tunnel diode performance. Jp and Jv are defined by the following equations.
where A is the cross-sectional of the diode, specified in units of cm2. Therefore, Jp has units of Amps/cm2.
Vp Vv I
1.2. RTD-FET for Logic and Memory Applications
The integration of RTDs with FETs, proposed by Seabaugh et al., has led to improved mixed-signal circuit (Fig. 1.3) and is currently being sought to produce THz
signal generation and detection. The comparator circuit implemented with
RTD-MODFET circuitry has a significantly smaller component count, taking 1/6 the area,
while outperforming the MODFET-only circuit in speed and power consumption [6-7].
Figure 1.3: Schematic diagram of an RTD-MODFET comparator circuit vs. a
MODFET-only comparator circuit, comparators designed for 35 GHz operation, indicating the reduction in component count and improvement in circuit speed. Adopted from Seabaugh .
With existing CMOS, the speed gap between microprocessor and memory is
increasing and memory access will become the limiting factor. Tunnel diode based
memory addresses this niche issue as well. Tunneling diode based SRAM, or T-SRAM,
speed of SRAM and puts it into the footprint of a DRAM cell by reducing component
count (1 transistor/2TDs versus 6 transistors) and uses a tunnel diode pair to store a bit
. The instability in the NDR region leads to bistability and the circuit latches to the
high or low state, thus storing information. This T-SRAM cell was demonstrated using
InP-based materials and showed considerable savings in power consumption.
0.0 0.1 0.2 0.3 0.4
9 x 10 10 x 10
Figure 1.4:. The schematic circuit diagram and I-V characteristic of a T-SRAM memory cell. Adopted from van der Wagt .
Up to the early part of 1990s, most of the work in tunnel diode development was
done in III-V compound semiconductors. Recent breakthrough in the development of
Si-based Resonant Interband Tunnel Diode (RITD) by Rommel et al., however, showed a promising potential in overcoming the compatibilities issues. The structures investigated
utilized undoped Si or SiGe layers sandwiched between two δ-doping planes grown by
MBE [9-10]. The latest SiGe design by Niu Jin et al. results in peak-to-valley current
ratio (PVCR) up to 3.6 with peak current density (Jp) up to 300 A/cm2 .
This thesis will be the first attempt to integrate SiGe RITD with CMOS
Si-based RITD-FET circuitry that will exhibit superior device performance for logic and
1.3. Organization of Thesis
The discussion is presented according to the progression of the idea, which is not
necessarily in chronological order. Chapter 2 discusses the fundamental physics and
mechanism of tunnel diode in general. It is followed by a discussion of the development
of Si-based resonant interband tunneling diode (RITD) given in chapter 3. The Si/SiGe
RITD is then used as a template for integration with CMOS. Chapter 4 reports the
integration strategy used in this investigation. The discussion includes the thermal budget
consideration, placement of RITD, mask layout design, and process development. The
anticipated process challenges were studied in greater detail in chapter 5. Moreover,
chapter 6 gives a detailed report on how the geometry and area affects the device
performance of RITDs. A new concept of integration by overgrowth method is
introduced in chapter 7. Finally, chapter 8 presents the result of the first successful
This chapter describes the fundamental theory behind the operation of tunnel
diode. Section 2.1 gives brief overview of quantum mechanical tunneling. Mathematical
expressions for tunneling probability for different potential barriers are given. The
discussion is then followed by description of three different classifications of tunnel
diodes. Section 2.2 details the operation of Esaki tunnel diode. Different current
components are discussed, and mathematical expressions are presented. It is not the goal
of this study to show rigorous mathematical derivation of equations presented in this
chapter. Rather, they are given to show the effect of some important parameters. Section
2.3 describes Resonant Tunnel Diode (RTD). Section 2.4 gives brief overview of
Resonant Interband Tunnel Diode (RITD), which will be explained in great detail in
2.1. Quantum Mechanical Tunneling
Many people have tried and debated how to accurately describe tunneling
phenomenon. However, there has not been one satisfying answer simply because the
concept has no analog in classical physics. Consider the case of a particle, such as
electron, traveling towards a finite potential barrier as illustrated in Fig. 2.1. In classical
physics, there is no possibility that it is ever being found on the other side of the barrier,
unless its kinetic energy exceeds the height of that barrier . Quantum mechanically,
beyond the boundaries of the barrier. In other words, there is a finite probability that the
particle slightly penetrates into the potential barrier for some distance. If the potential
barrier is thin relative to the particle’s Bloch wavelength, the particle can slip freely
through the barrier without having the energy to surmount it. This ghostlike passage
through a barrier is known as quantum mechanical tunneling .
Figure 2.1: Schematic diagram showing the tunneling of an electron or similar particle from the left of the potential barrier of thickness L and height V0, which is
greater than the incident particle energy. Adopted from McKelvey .
The rectangular potential barrier as shown in Fig. 2.1 is most appropriate to model
the RTD. Interband tunnel diode, however, are often modeled as to have either triangular
or parabolic potential barrier (Fig. 2.2). Tunneling probability can be approximated using
Wentzel-Kramers-Brillouin (WKB) method as in the case of triangular (Eq. 2.1) and
Figure 2.2: (a) Triangular potential barrier; (b) parabolic potential barrier. Adopted from Sze .
3/ 2 4 2 * exp
m E T
1/ 2 3/ 2
m E T
where, m* is the effective mass of the particle, Eg is the bandgap of the semiconductor, ħ
is the Planck constant, and ξ is the electric field. From both expressions it is clear that to
obtain large tunneling probability, both the effective mass and the bandgap should be
small and electric field should be large.
In summary, the necessary conditions for tunneling are: (1) occupied energy states
exist on the side from which the electron tunnels; (2) unoccupied energy states exist at
the same energy levels on the side to which the electron can tunnel; (3) the tunneling
potential barrier height is low and the barrier width is thin enough that there is a finite
2.2. Esaki Tunnel Diodes
The introduction of junction transistor in the early 1950s stimulated a rigorous
investigation to understand p-n junction properties . Special interest was directed
towards different types of breakdown mechanism. One mechanism being postulated was
avalanche breakdown, in which tunneling occurs from the valence band in the p+ type
region to the conduction band in the n+ type region. Further investigation showed that the
breakdown voltage decreases substantially as the net impurity density of one side of the
diode increases to the order of 1017 cm-3. Building upon these findings, Esaki
experimented with even higher doping concentration. He observed that when the doping
level exceed 1018 cm-3 the breakdown voltage became much less than 1 V and the reverse
bias current became more conductive then the forward direction, a device referred to
these days as the backward diode. He was compelled to increase the doping concentration
on both sides of the junction that led to the invention of tunnel diode. Tunneling current
was observed at very low forward bias voltage. He also reported a unique negative
differential resistance behavior. To honor his discovery, this type of diode is often
In other words, Esaki tunnel diode consists of p-n junction, in which both p and n
are degenerately doped. Fig. 2.3 shows a schematic energy diagram of a tunnel diode in
thermal equilibrium. Because of the high doping concentration, the Fermi energy level is
a few kT above the conduction band in n+ side, and few kT below the valence band in the p+ side. The width of depletion region is typically of the order of 10 nm or less, which is
substantially narrower than the conventional p-n junction.
Fig. 2.4 shows the energy band diagram with the corresponding I-V characteristic
under different biasing conditions. When the junction is in reverse bias (Fig. 2.4(a)),
tunneling occurs from the occupied states in p side to available states in the n side. At
zero bias or thermal equilibrium as in Fig. 2.4(b), there is no available state for tunneling
to occur; thus, no current flows. When small forward bias is applied (Fig. 2.4(c)) the
filled states on the n side can tunnel to the unoccupied states in the p side, resulting in
sudden rise in current. Tunneling continues to occur until the conduction band of the n
side cross the valence band of the p side. Biasing slightly beyond this condition results in
abrupt decrease in tunneling probability, leading to sudden drop in current. Negative
differential resistance (NDR) behavior is observed. When the bias exceed the built-in
potential of the junction, the diffusion current dominates, resulting in exponential
increase in current.
Based on the band diagram analysis, the static IV-characteristic of a tunnel diode
can be broken down into three different current components: (1) band-to-band tunneling
current, Jt, (2) excess current, Jx, and (3) thermal current, Jth, . total t x th
Figure 2.4: Schematic energy band diagram of tunnel diode in: (a) reverse bias; (b) thermal equilibrium or zero bias; (c) to (d) different stages of forward bias conditions; (e) the corresponding I-V characteristic.
To the first order approximation, tunneling current can be derived using the density states
in the conduction and valence bands. Assuming parabolic potential barriers (Eq. 2.2) and
taking into account the conservation of momentum, tunneling current is given as
1/ 2 3/ 2
exp ( ) ( ) exp
2 2 2
p C V
m E E
J F E F E dEdE
E q π π ξ ⊥ ⊥ = − − −
∫h h 144424443 (2.4)
where FC(E) and FV(E) are the Fermi-Dirac distribution function, E┴ is the energy
associated with the momentum perpendicular to the direction of the tunneling. It is (c) (d) (e) (a) EFn ECn EVn ECp EFp EVp (b) a
c d e
important to note at this point that Jt is clearly direction proportional to tunneling
Figure 2.5: Three current components of static I-V characteristic of tunnel diode: band-to-band tunnel current, excess current, and thermal current. Adopted from Sze .
The second component is known as excess current. In an ideal case, the tunneling
current should cease to zero when the conduction band of n-side start to overlap the
valence band of the p side. In practice, however, the current has never reach zero, and the
current is considerable in excess of the normal diode current; thus, the term excess
current . It was suggested that this excess current can be accounted for by a
mechanism of carriers tunneling by way of energy states within forbidden gap.
Chynoweth et al. proposed a mathematical model of this current based on the different possible routes through which electron can tunnel (Fig. 2.6). The expression for excess
current is given as follows.
1 exp 0.6
x x x g n p
J = A D −α E −qV + V +V (2.5)
Finally, the thermal current is the familiar normal diode current.
exp exp 1
qV J J
Figure 2.6: Mechanism of tunneling via states in the forbidden gap for the excess current flow. Adopted from Chynoweth .
Table 2.1 lists different Esaki tunnel diodes. It is important to note that the first
three studies on the list were using alloying process to fabricate tunnel diodes. In later
discussion in chapter 3, this technique posts a problem for large scale integration with
Table 2.1: Examples of reported Esaki tunnel diode results for various materials. The entries listed in the table list the highest reported experimental values in each system. Adopted from Rommel .
Study Material Jp (kA/cm2) PVCR
Meyerhofer, 1962 Ge 16 9.3
Franks, 1965 Si 1 3.8
Holonyak, 1960 GaAs – 25.0
Richard, 1993 P+GaAs/P+In0.1Ga0.9As/
2.3. Resonant Tunnel Diodes
Another type of structure that falls under the classification of tunneling device is
Resonant Tunnel Diodes (RTD). The mechanism in which the device operates bears little
resemblance to the conventional diode or even to Esaki diode. RTD is a unipolar device
as compare to Esaki diodes that is bipolar. In other words, there can only be p-type or
n-type RTD. This also means that tunneling mechanism occurs on the same energy band;
hence, it is sometimes referred as resonant intraband tunnel diode. In order to appreciate
the technology, let’s consider some conceptual basis in quantum mechanics.
It is well understood that electron bound to a potential well with finite width and
height, or quantum well, can no longer have continuous every spectrum; rather, it
develops discrete energy levels [12,16]. Fig. 2.7 shows the first three of energy levels in
which electron can exist and oscillate within the well. This phenomenon is being
exploited in the design of RTD.
Potential wells can be formed by a pair of heterojunctions, which produce large
conduction band offset in the case of n-type RTD. This concept has been realized by
using non-equilibrium epitaxial processing technique such as molecular beam epitaxy
(MBE). Such technique has the capability of growing epitaxial thin film of different
materials to the order of atomic layer.
Fig. 2.8 shows the energy band diagram of a double barrier RTD and the
corresponding IV characteristic at different bias conditions. The width of the barrier has
to be thin enough to allow an appreciable probability of tunneling. The height can be
engineered by choosing different wide-bandgap materials and typically is greater than
1V. Tunneling occurs when energy of electrons at the electrode coincide with the energy
level in the confined states within the well . This condition is known as resonance. At
zero bias (Fig. 2.8(a)) there is no available states in the well; hence, no current flows.
When a small forward bias is applied, the energy levels inside the well are lowered in
such a way that resonance occurs (Fig. 2.8(b)). Electrons now can tunnel from the left
electrode to quantum states within the well, and subsequently tunnel the right electrode,
resulting in tunneling current. Biasing slightly beyond the critical voltage, the diode is no
longer in resonance, leading to sudden decrease in current and NDR behavior is observed
in the IV characteristic. Further biasing will eventually provide electron enough kinetic
energy to surmount the potential barriers, cause the current to rise again.
Table 2.2 lists different RITDs. One of the greatest issues in the RTD is that it can
produce high excess current at room temperature if the quantum wells are not sharply
defined or phonon excitation is required for energy conservation. Most of RTD
Figure 2.8: (a) RTD at zero bias. (b) Small forward bias is applied, creating resonance condition so that tunneling occurs. (c) Biasing beyond critical voltage results in NDR behavior. (d) The corresponding static IV characteristic. Adopted from McKelvey .
Table 2.2: Examples of reported RTD results for various materials. The entries listed in the table list the highest reported experimental values in each system.
Adopted from Rommel .
Study Material Jp (kA/cm2) PVCR
Ismail, 1991 Si/Si0.7Ge0.3/Si 0.4 1.2
Kan, 1988 AlAs/GaAs/AlAs on Si 1.63 2.9
Brugger, 1991 AlGaAs/GaAs/AlGaAs 10 7.2
Chow, 1992 AlAs/In0.53Ga0.47As/AlAs 76 25
Smet, 1992 AlAs/In0.53Ga0.47As/InAs/
Muto, 1994 AlAs0.56Sb0.44/In0.53Ga0.47As/
2.4. Resonant Interband Tunnel Diodes
Resonant interband tunnel diode (RITD) is a hybrid between Esaki diode and
RTD. It incorporates quantum wells on each side of p-n diode structure. The conceptual
idea was first proposed by Sweeny and Xu in the late 1980s . They suggested three
different configurations of RITD. Fig. 2.9 shows one the proposed structures.
Fundamentally, RITD is a double well bipolar device as to compare to RTD, which is a
double barrier unipolar device. As forward bias is applied to the device, resonant
tunneling occurs between holes states in the p side quantum well and electron states in
the n side quantum well. Beyond the critical voltage, the diode is no longer in resonance,
and NDR will occur. Like in the case of Esaki and RTD, further biasing will give carriers
enough energy to overcome the potential barriers, resulting in exponential increase in
Figure 2.9: Schematic energy band diagram of proposed RITD. Heterojunctions forms quantum wells on conduction and valence bands. Adopted from Sweeny and Xu .
Another configuration that is most relevant to the study presented in this thesis is
the modulated-doped RITD. Fig. 2.9 shows the schematic energy diagram of such device.
One of the advantages is that the pn diode does not have to be degenerately doped in
favor of ultrahigh speed performance due to lower junction capacitance. The quantum
well on both side of the junctions can be realized by incorporating two delta doping
planes. This structure was first demonstrated by Rommel et al.  on Si/SiGe/Si using δ
-doped plane of B and Sb. The development of Si-based RITD will be discussed in detail
in Chapter 3. Finally, Table 2.3 list examples of different RITDs.
Figure 2.10: (a) Schematic band diagram of a modulation-doped RITD. Quantum well on both side of the diode can be formed using two delta planes. Adopted from Sweeny . (b) Discrete energy levels in δ-doped plane. Adopted from Gossmann .
Table 2.3: Examples of reported RITD results for various materials. RITD type refers to configurations defined by Sweeny. Adopted from Rommel .
Study RITD Material PVCR
Su, 1993 III GaAs/δn+-i-δp+ 5.0
GaAs/δn+-i-δp+-i δn+ 3.2
Duschl, 2001 III Si/δp+/SiGe/δn+/Si 6.0
Chen, 1990 II InAs/AlSb/GaSb 4.7
Shiralagi, 1997 II InAs/AlSb/GaSb 1.1
Shiralagi, 1998 II InAs/AlSb/GaSb 15.0
Soderstrom, 1989 Double Barrier InAs/AlSb/GaSb/AlSb/InAs 20
Day, 1993 Double Barrier p-n InAlAs/InGasAs DQW 104
This chapter gives an overview of Si-based Resonant Interband Tunnel Diode
(RITD) technology. The chapter is organized in two sections. The first section traces the
chronological development of Si-based RITD up to the present time. The second part of
the chapter describes the fabrication and process challenges of discrete SiGe RITDs.
3.1. Historical Development
In 1993, Jorke et al. demonstrated for the first time epitaxially grown Si-based interband tunnel diode . The original intention of the experiment, however, was not to
study tunnel diode per say; rather to investigate the defect assisted tunneling current at p-n junction epitaxially grown by using MBE technique. His approach was to insert a thin i -layer of different thickness forming p+in+ junctions. He discovered that for i-layer thickness of 5 nm, the IV characteristic showed negative differential resistance (NDR)
behavior with peak-to-valley current ration (PVCR) of 2 at room temperature.
Unfortunately, this work was overlooked by the scientific community as the context of
overall paper was on bipolar junction transistor (BJT).
Four years prior to Jorke’s experiment, a new concept of resonant interband
tunneling diode was introduced by Sweeny and Xu  as discussed in the previous
chapter. The embodiment of this idea in Si-based material, however, was not realized
until 1998 through a study conducted by Rommel et al. [9,10] using δ-doped planes and
doped injectors, (iii) off-set of the δ-doping planes from the heterojunctions interfaces,
(iv) low temperature molecular beam epitaxial growth (LT-MBE), and (v) post-growth
rapid thermal annealing (RTA) for dopant activation and point defect reduction.
Figure 3.1: Schematic diagram of the first Si/SiGe/Si RITD structures. (a) Tunneling barrier was 4 nm Si0.5Ge0.5. (b) Additional 1 nm of undoped on either side of
Si0.5Ge0.5 was utilized as tunneling barrier. (c) The schematic energy band
diagram of structure TD2. (d) IV-characteristic of TD2. Adopted from Rommel .
It was theorized that i-layer would reduce the total number of scattering sites in the tunnel barrier which may contribute to excess current, enhancing the PVCR. Secondly
it also provides a buffer for the interdiffusion of dopants. Si0.5Ge0.5 was chosen as the
the potential barriers; hence, increases the probability of tunneling as Eq. 2.1 and 2.2
The effect of post-growth RTA temperature was also studied. Samples as-grown
showed no evidence of NDR. In contrast, samples that went under hear treatment at
700oC and 800oC for 1 minute, exhibited NDR behavior. In addition, PVCR and peak
current density (Jp) were found to be strongly dependent on the placement of δ-doped
planes. Devices with TD2 structure show superior performance with a PVCR up to 1.54
and Jp of 3.2 kA/cm2.
Encouraged by the findings, Rommel and his team made further modifications to
the device structure by varying the spacer thickness and optimizing post-growth RTA
temperature . They demonstrated PVCR as high as 2.05 and Jp of 22 kA/cm2 for
spacer thickness that consist of 2 nm of Si0.5Ge0.5 sandwiched between 1 nm of
Furthermore, they also experimented on spacer made of undoped Si. The key
difference between purely Si RITD and SiGe RITD are: (1) purely Si tunnel barrier
eliminates critical thickness issues and strain associated with SiGe alloys, (2) strain
relaxation during the RTA heat treatments is avoided, and (3) quantum confinement is
not aided by the presence of a heterojunctions discontinuity . This particular study,
however, did not result in any improvement in device performance. The highest PVCR
obtained was 1.41 with Jp of 10.8 kA/cm2.
Adopting the structure proposed by Rommel (TD2), Duschl et al. at Max Planck
Institute in Germany replicated the experiment . They demonstrated a PVCR of 4.2
better growth condition. The device performance was further enhanced by varying Ge
content in the i-layer as to form Si0.52Ge0.48 and adjusting its position within the intrinsic
zone. They reported PVCR as high as 5.45 with Jp or 8 kA/cm2 . In a third
experiment, a new world record was achieved with PVCR of 6.0 and an extremely high Jp
of 33 kA/cm2 by substituting the element of n-type δ-plane with P rather than Sb. .
Fig. 3.2 summarizes the latest result from Duschl’s group.
Figure 3.2: (a) IV characteristic of different annealing temperature for structure consisting δB/3nm Si0.54Ge0.46/1 nm Si/δP. (b) The corresponding Jp, Jv, and
PVCR. Adopted from Eberl .
Continuing Rommel’s efforts and gaining insights from Duschl’s work, Niu et al. immediately employed the δ-doping plane of P . They observed right away a
substantial enhancement in PVCR from 2.05 to 2.7. Phosphorous has higher
solid-solubility limit than Sb at the growth temperature, resulting in higher degeneracy at the δ
-doped layer and increase in tunneling probability. Recent study that utilized SiGe
cladding layer to suppress B diffusion during the post-growth anneal (Fig. 3.3) shows a
PVCR as high as 3.6 and a Jp of 0.3 kA/cm2. The new structure is shown to have higher
optimum annealing temperature, which appears to be more effective in reducing defects
this technology more attractive for integration with current CMOS technology. For this
reason, Niu’s latest structure will be utilized in this thesis work. Finally, table 3.1 list the
development of RITD.
Figure 3.3: (a) Schematic diagram of RITD with SiGe cladding layers to suppress B diffusion. (b) Schematic energy band diagram of the corresponding structure. (c) The solid line represents the IV characteristic of structure in (a). Adopted from Niu .
Table 3.1: Chronological development of RITD technology.
Study Description Jp (kA/cm2) PVCR
Sweeny, 1989  Conceptual design using
δ-doped planes – –
Rommel, 1998  δB/i-Si/Si0.5Ge0.5/i-Si/δSb 22.0 2.05
Duschl, 1999  δB/i-Si/Si0.5Ge0.5/i-Si/δSb 3.0 4.2
Duschl, 1999  δB/i-Si/Si0.52Ge0.48/i-Si/δSb 8.0 5.45
Eberl, 2001  δB/i-Si/Si0.52Ge0.48/i-Si/δP 33.0 6.0
Niu, 2002  Si Ge 4/δB/ Si Ge /i-Si/δP 0.3 3.6
100nm n+ Si
2nm undoped Si 4nm undoped Si 0.6 Ge 0.4
80nm p+ Si
P δ-doping plane
B δ-doping plane 1nm undoped Si 0.6 Ge 0.4
0.0 0.1 0.2 0.3 0.4 0.5 0.6 0.7 25 50 75 100 125 150 175 200 225 250 275 300 325 350
0/4/2 spacer with cladding layer PVCR = 3.6
0/4/2 spacer PVCR = 3.0
1/4/1 spacer PVCR = 1
Cu rr en t D e ns ity ( A /c m 2 ) Voltage (V)
3.2. Fabrication Processes and Challenges
In theoretical analysis of a device, an ideal case is usually assumed. It only takes
the consideration of nature limiting conditions, such as the band gap of a material or
effective mass of a certain particle. In reality, there are many other limiting factors that
can only be determined experimentally. In many cases, these non-ideality factors can be
traced to processing issues and limitations. The following sub-sections will discuss the
fabrication of discrete SiGe RITD in sequential order from substrate preparation to
3.2.1. Substrate Cleaning and Preparation
Substrate preparation is the first critical step prior to any epitaxial growth process.
Since the grown epi-layer tends to adopt the crystal structure of the underlying substrate,
the presence of native oxide or other impurities on the surface are undesirable. Therefore,
the removal of these interfacial films need to be performed before successful epitaxial
growth can be initiated .
The goal is to produce a hydrogen-terminated surface that is stable in air for
several hours. A cleaning technique known as “Shiraki” process has been widely used
and accepted by Si-MBE community as a standard method. The process, however,
involves many steps and requires high temperature treatment at 850oC prior to growth.
Thompson et al. developed a simplified version of the Shiraki process (Table 3.2) that
requires lower temperature treatment at 200oC. This cleaning process is usually used in
Table 3.2: Abbreviated Shiraki cleaning process develop at Naval Research Laboratory. Adopted from Thompson .
HF DI H2O rinse
Boiling HNO3 for 10 min.
DI H2O rinse
4% HF for 20 sec. DI H2O rinse
Boiling NH4OH: H2O2:H2O (1:1:3) for 10 min.
DI H2O rinse
4% HF for 20 sec. Dry N2
Thermal steps prior to MBE growth 200oC for 1 hr. bake
Ramp to buffer growth temperature, 650oC
3.2.2. Low Thermal Molecular Beam Epitaxy (LT-MBE)
The fabrication of RITD layers is based on the solid-source molecular beam
epitaxy (MBE) technique. The discussion in this section starts with a general description
of epitaxy process and will shift to LT-MBE gradually.
By definition, epitaxy is a process of growing a crystalline material upon a
crystalline substrate. If the grown material is identical with the substrate, it is termed
homoepitaxy. In the case of different materials is referred as heteroepitaxy. Since
dissimilar materials have different lattice spacing, there is usually some amount of strain
associated with heteroepitaxy. In the case SiGe grown on Si substrate, there is about 4%
lattice mismatch in which the Si has wider lattice constant.
There are several requirements for successful heteroepitaxy process . First,
and preparation. Moreover, there must be chemical compatibility between materials to
avoid compound formation or massive dissolution. Finally, the grown material and
substrate should have closely matched thermal expansion coefficient to avoid dislocations
on the interface.
Film formation is initiated by nucleation process by which reactants combine to
form isolated ensembles that attach to different points on the surface of the substrate. Fig.
3.4 illustrates different possible sites of nucleation in cubic crystal with their associated
binding energies. The cube is bounded to their neighbor with a binding energy of φ1/face
and φ2/edge. Upon the arrival on the substrate (site A), species move by surface diffusion
mechanism until they find nucleation sites or being desorbed from the surface. The
probability of desorption is higher on the sites with lower binding energy; hence,
nucleation is likely to happen on steps and corners (site B and C respectively). Any
presence of crystal defects, contaminants, and abrupt topography can be preferable
Site A: Adsorption on a surface, with a binding energy of φ1 + 4φ2.
Site B: Adsorption at a step, with a binding energy of 2φ1 + 6φ2.
Site C: Adsorption at a corner, with a binding energy of 3φ1 + 6φ2.
Site D: Adsorption incorporation into a step, with a binding energy of 4φ1 + 8φ2.
Site E: Adsorption incorporation into volume crystal, with a binding energy of 6φ1 + 12φ2.
MBE is one of the techniques to grow epitaxial layer. Fig. 3.5 shows the typical
configuration of an MBE tool. Material to be grown is directly transported to the
substrate by a directed molecular beam under ultra high vacuum system. The beams of
dopant, such as B and P, are generated by thermal evaporation of their solid forms. Si,
however, requires electron beam heating to produce significant flux of material. The
growth rate, in which proportional to the incoming flux, is controlled by mechanical
shutters. A very well controlled growth rate down to 1 Å/sec can be achieved. In addition,
the substrate temperature is usually elevated to assist surface diffusion, resulting in better
Figure 3.5: Basic configuration of an MBE tool. Adopted from Ghandhi .
The incorporation of δ-doped planes in RITD structures posed a major challenge.
By definition δ-doped plane is a region of doping impurities within a two dimensional
with only flux of dopant atoms onto the substrate. The formation of δ-Sb or δ-P is often
limited by phenomenon known as segregation, which occurs when impurities exceed the
solid solubility limit in Si, leading to higher surface concentration. The direction in which
the dopant segregate is towards the direction of the growth, resulting in broadening of δ
-Sb dopant profiles. On the other hand, the growth of δ-B is often characterized by
diffusion that also results in the undesirable of broadening of the dopant profile.
The problem of Sb and P segregation can be overcome by lowering the growth
temperature, allowing the dopant atom to have enough energy only to impinge into the
crystal lattice immediately after its arrival. The trade-off, however, low temperature MBE
process usually results in higher defect density. In the case of δ-B, although LT-MBE
may help to form a sharper dopant profile it is still vulnerable to the effect of post-growth
thermal treatment. Finally, Table 3.2 describes a typical step-by-step LT-MBE growth of
SiGe RITD used in this thesis work.
Table 3.3: LT-MBE process to fabricate SiGe RITD structure as described in Fig. 3.3 (a). Process recipe is courtesy of Phillip E. Thompson.
Layer Si growth rate (Å/sec) Ge growth rate (Å/sec) Temp. (Substrate oC) Thickness (Å)
Si buffer 1 – 650 20
p+Si 1 – 650-500 100
p+Si 1 – 500 540
p+Si 0.6 – 500 160
SiGe 0.6 0.4 500 10
δ-B plane – – 500-320 –
SiGe 0.6 0.4 320 40 Si 0.6 – 320 20
δ-P plane – – 320 –
n+Si cap 1 – 320 1000
3.2.3. Post-growth Rapid Thermal Anneal
Thermal treatment post MBE growth is proven to be necessary, and the process is
often referred as post-growth anneal. As grown RITD usually doesn’t exhibit NDR
behavior or very small PVCR in the IV characteristic. The reason is that the dopant,
which are impinged on the silicon, are only interstitially incorporated into the lattice
structure; hence, they are not electrically active. An external thermal energy allows the
dopant to move around and lodge into the Si lattice by substitution mechanism, producing
Moreover, the post-growth anneal also helps to eliminate point defects that are
formed during MBE growth due to strain associated with different layers and amount of
impurities. As a result, the tunneling assisted current through defects sites will be
substantially reduced, lowering the valley current and increasing PVCR. The higher the
post-growth anneal temperature, the more effective it dissolves the defects. This
enhancement, however, is limited. Higher anneal temperature will also result in the
broadening of the δ-doped profile, which in turn deteriorates the PVCR.
Since the goal is to preserve the integrity of δ-doped planes, rapid thermal anneal
(RTA) is needed. Fig. 3.5 shows the schematic diagram of typical RTA system. A
well-controlled spike of high temperature for a short amount of time can be achieved.
In summary, the optimum post-growth anneal condition is achieved when (i)
dopant activation is maximized, (ii) the number of defects sites are minimized, and (iii)
the broadening of dopant profile due to either diffusion or segregation is minimized. In
the experiment conducted by Jin et al. , they observed that the anneal condition is
suppress boron diffusion as shown in Fig. 3.6(a). Consequently, the thermal budget is
also raised, and the optimum anneal condition is achieved at 825oC for 1 minute.
Figure 3.6: Schematic diagram of typical RTA system. Adopted from Ghandhi .
6 8 10 12 14 16 0 2 4 6 8 10 12 14 Si Si
Boron Delta Plane
SiGe SiGe B concen tr ation (1 0 19 cm -3 ) Position (nm) no SiGe
SiGe on the right side SiGe on both sides
650 700 750 800 850
1.0 1.3 1.5 1.8 2.0 2.3 2.5 2.8 3.0 3.3 3.5 1/4/1 spacer 0/4/2 spacer
0/4/2 spacer w/ cladding
RTA Temperature (o C)
3.2.4. Patterning and Metallization
Prior to metallization, native oxide layer that may have been grown through
exposure to room air is removed by a short buffered oxide etch. This step is critical as to
guarantee lower contact resistance. A thin layer of Ti/Au is then deposited using thermal
evaporation technique. Circular dots of various sizes are patterned using the conventional
contact lithography. Using the Ti/Au dots as self-aligned etch mask, the unwanted Si
epitaxy regions are removed using wet etch in HF:HNO3:H2O (1:100:100) solution. The
etch rate is found to be strongly dependent on the amount of HF in the mixture, and is
calibrated in such a way to be around 100 nm/min. Finally, a layer of Ti/Au is also
The integration of SiGe RITD into CMOS technology will require modification to
the existing CMOS fabrication steps. The goal is to minimize the addition of process
steps while maintaining the integrity of CMOS devices. This chapter will address many
different aspects of the integration process. Section 4.1 describes the integration strategy
employed in this study. Section 4.2 will discuss the testchip design and fabrication.
Moreover, section 4.3 lists the complete fabrication processes from start to finish.
4.1. Integration Strategy
The integration strategy used in this thesis work involves primarily two aspects:
thermal budget and the placement of RITDs within CMOS template.
4.1.1. Thermal Budget
The limiting condition of a thermal process is often referred as thermal budget. At
high temperature, dopant will have enough energy to redistribute in the crystal lattice
through either interstitial or substitutional sites; hence, changing the electrical property of
the material. The velocity by which the dopants move at a specific temperature is defined
as diffusivity (D) with unit of cm2/second. The square root of the product of D and time
(i.e. Dt ) is known as diffusion length, which is used to determine the thermal budget of a process. Exceeding a thermal budget will result in substantial alternation in device
In the effort to integrate SiGe RITD and CMOS, the thermal budget of each
technology will be considered carefully as shown in Table 4.1. In CMOS, the step from
well to source and drain formation is often referred as the front-end processes. Likewise,
the subsequent processes, such as passivation and metallization, are called back-end
processes. It is obvious that the thermal budget of RITD is much less than the CMOS
front-end processes and higher than the back-end processes. Therefore, it is evident to
build the RITD after all CMOS front-end steps, but prior to the back-end.
Table 4.1: Thermal budget of CMOS and RITD. The CMOS process is based on the
twin-well CMOS technology developed at Rochester Institute of Technology.
Critical Steps Temp(oC) Critical Steps Temp(oC)
Well drive-in 1100 MBE Growth 320-650
Field oxide growth 1100 Post-growth anneal 825
Gate oxide growth 1000
Poly gate deposition 610
S/D anneal 1000
Metal sintering 415
4.1.2. The Placement of RITD within CMOS Template
The most suitable place to build the RITD was right on top of the source/drain
(S/D) of CMOS devices as shown in Fig. 4.1. This configuration shows
three-dimensional structuring where one device is integrated vertically on top of the other.
There are many advantages to this strategy. First, compact circuit that requires less area
with greater functionality can be achieved. Secondly, there is possibility that S/D and
RITD can formed in a single MBE growth, featuring RITD on raised S/D stacks. In order
Figure 4.1: Schematic diagram of RITD built right on top of S/D of FET device. Adopted with modification from Seabaugh .
The goal of this study is to prove the concept that it is feasible to monolithically
integrate RITD and CMOS on the same substrate. Therefore, there is no immediate need
to build RITD right on top of the S/D regions. Instead, RITDs would be grown on
separate regions, which have been implanted with identical condition as the S/D of
PMOS as shown schematically in Fig. 4.2.
Figure 4.2: RITD grown on regions that have been implanted with identical condition as P+S/D of PMOS.
100nm n+ Si
2nm undoped Si 4nm undoped Si 0.6 Ge 0.4
80nm p+ Si
P δ-doping plane
B δ-doping plane 1nm undoped Si 0.6 Ge 0.4
P+ N+ N+ P+ N+ P+
P+ implant FOX
CVD Ox CVD Ox
Metal CVD Ox
NMOS PMOS RITD
Poly Gate Poly Gate
Gate Oxide Gate Oxide